The mechanism of processes on the interphase boundary of the passivating oxide layer PL has a fundamental value, whereas, the properties of the passivating layer are determined by them.In this paper a consistent model of the boundary metal-oxide MO is presented.
General stationary laws.
On the interphase boundary of metal with PL, the continuous dissolutionof metal occurs.it disappears consecutively monolayer after a monolayer and the cells of oxide occupy its place. if at time t the layer of metal M of thickness x disappears, then the plane MO displaces in its side with the speed
An International Open Free Access, Peer Reviewed Research Journal CODEN: OJCHEG
2014, Vol. 30, No. (2): Pg. 661-665
A Physical Model of the Interphase Boundary of the
Passivating Layer on the Metal in the Electrolyte Solutions
SAIF A. MOUHAMMAD* and AYMAN F. AMER
Department of Physics, Taif University, Saudi Arabia. *Corresponding author E-mail: firstname.lastname@example.org
(Received: March 01, 2014; Accepted: March 27, 2014)
The model of processes on the interphase boundary metal- passivating layer is proposed. The balance of ions upon the formation of the cells of oxide is examined. The velocity expressions of these processes are obtained.
Key words: Physical model, Passivity of metals, Electrolyte.
where ib- total dissolution current; µ, - the molar mass and density.The thickness of the oxide layer ok, substitutingfor the same time, is also equal.
Thus, the surface MO serves as the source of ions Mz+
ok, and in the passivating layer, their
intensive transfer by the mechanism of hopping migration in the strong electric field E should be occurred. Accordingly, the total current of the dissolution of metal is divided into the transfer current ibm of the ions through the boundary MO in PL and the current ibo of oxide formation on this boundary (subscripts indicate: b- boundary, m-metal, o- oxygen; the current ibo determines a quantity of metal ions, which in 1cm³ every second are connected in the layer M with oxygen), such as
The subsequent analysis confirms this conclusion. The total current must be equal
Where am - interatomic distance in the cationic sublattice, ab - transfer coefficient on the boundary MO.
Equation(3) assumes, that an ionM,
passing into the state of anion , must overcome a potential jump M=aME .Thus, the barrier of transition decreases to WM=abzMM. The constant of transition speed is determined from the independent temperature measurements ( for Fe, for example, ).
The total current ib is the fundamental characteristic of stationary processes on the interphase boundary MO, and the micro scheme of the formation of cells M2O3 are ambiguous. They must consider a difference between the interatomic distances and the angular directions in the lattices of metal and oxide, and require the use of probabilistic methods for describing regrouping particles.
Further, it is interesting to detail a physical
situation on a surface MO to calculate the currents ibm, ibo and the ratio between the values N1 and N2. For this purpose let us proceed from general consideration to the specific models of processes on the boundary MO.The most simple and real vacancy model is presented below. It allows to open a better physical sense of therelations (3).
The vacancy model of MO boundary
Vacancy model proceeds from the idea about the fact that, for forming the new cell M2O3, three ions O
2-ok from the passivating layer must
penetrate in the boundary monolayer of metal. This requires the presence of three vacancies VM in it, which can arise only as a result of previous transition in the passivating layer of three ions of metal. These ions fill three vacancies Vom in the cation’ssublattice of oxide. The transition scheme (VM- vacancy in a metallicsublattice of oxide,- vacancy in the boundary layer of the metal M )
Transition (4) serves as the necessary condition for the subsequent penetration into the layer of oxygen ions
Where Vok- vacancy in the oxygen
sublattice in place passedinto the metal ion O 2-ok.
The opposite reactions (4), (5)- appear basic in the vacancy model. It is obvious, that the surface MO serves as a drainof cationic vacancy Vom, brought by their diffusive flow jmv from solution. Simultaneously, it is the source of the vacanciesVom, which are discharged into the solution by their flow jov. Flows jmv and jov appear, of course, as a result of the motion of ions Mz+
ok and O
2-ok in the passivating
layer by the mechanism of hopping migration in the strong field.
in this transformation, the vacancies Vm are mediators, which connect processes (4) and (5). Their total quantity is determined by the withdrawal of metal ions and penetrationin metal of the oxygen ions O
2-ok, i.e. the relations of the speeds (4) and
(5).In the stationary mode, the value of is invariable ( see below).
The speeds of formation of oxide and cation transfer through the boundaryMO.
Thus, processes On the boundary MO are characterized by the currents (speeds) ibm,ibo of reactions (4), (5) ibm,ibo and by the total current ib of the metal dissolution.It is measured, and is primary value, and its determination (3) can be called extra-model. The calculation of currents ibm,ibo depends on model presentations. let us examine these values.
1) Transition current ibm of ions M in the
passivating layer andtheir further transfer to the solution depends on the electric field E and the boundary concentration amNmv2 of vacancies Vom. Indeed, for transition into the passivating layer according to the scheme (4), ions M must cross the plane MO and move away from it on interatomic
distance am of a cationic sublattice, having
overcome potential jump m=mE . Transition barrier is reduced on Wm=bzmamE, its probability is proportional to a quantity of vacant places, i.e., the concentration amNmv2 of vacancies Vm. As a whole the speed (4) is equal
b- transfer coefficient , Nmet- concentration of atoms
in metal, - speed constant of reaction.
2) The current ibo of ions M, which form oxide MOz/2according to the reaction (5) , represents the speed of oxide formation on the Boundary MO.let
us take it equal to ( - constant of speed, reverse
current is neglected)
In the system (7), the dependence of current ibo on the field E, the concentration cmet, the vacancies Vm and the probabilistic factor f(u) are taken into account. the influence of field is regulated
by the value of transfer coefficient , and it is connected with the fact, that for the penetration into the metal through the plane MO, ion O
dislocate in the anion sublattice to the interatomic
distance ao, overcoming the potential jump
o=aoE.In this case, the barrier of penetration is reduced to the value Wo=abzoaoZ. Influence on current ibo of concentration cmet is considered with the fact, that without vacancies Vm, penetration can’t occur (see (5)).
The Probabilityfactor f(u) in (7) takes into account the specific mechanism of formation of cells MOz/2. If the penetration of ions and the structuring of cells occur in parallel, then it is not possible to exclude the deceleration necessary of regrouping of particles. The micro schemes of these processes can be different and random. Their possible influence on the speed of formation of oxide is described by probabilistic factor f(u) in (7). Its calculation is an autonomous task.
If the penetration of ions O
2-ok is limited
and it is weakly dependent on the subsequent
u 1 f
. Within the limit of the passivating layer it can consist of the partially structure systems complexes M2O3, the speed of formation of which is determined by (7) at f(u)=1. Str uctur ing depends, in par ticular, on the noncoincidence of interatomic distances and angular orientations in the lattices of metal and oxide.
gomogennmedium . However, in a
thin passivating layer on the strange base layer, these values b and b are not proved. Furthermore, the current values b,b in the volume of the passivating layer, and its more disordered boundaries may differ, i.e they depend on coordinate system. Apparently, in this respect, the boundary MO is isolated, on which exactly =b,=B. Then the jumps of the potential m and o overcome by ions M and O
2-okupon transition through the plane
MO are equal respectively to m=amE and m=aoE.
Barriers(4) in the Boundary MO are reduced on Wm = abzmm and. All this are taken into account in (6) and (7).
Using (6), (7) it is possible to calculate stationary concentration of vacancies. Actually, the withdrawal of ions M and the penetration of ions O
2-ok are strictly compensated (for example, for
formation M2O3, three ions M have to leave metal and three ions O
2-ok will penetrate in it).
for example, for forming , three ions must leave from the metal and three ions will penetrate in it.Therefore, speeds (6) and (7) are identical, i. e.
bo bm i
2 and, consequently (excluding small reverse
3) total current in ib the vacancy model is easy to relate with the values ibm and ibo taking into account, that the dissolution of the metal at the interface MO is fasteroxide formation. Actually, according to the presented above, for the appearance of a cell M2O3 it is necessary for emergence of a cell, that: a) three ions of metal from a layer M passed to PL by the scheme (4), composing the current ibm; b) three ions from a passivating layer enetrated into a layer according to the scheme (5); c) since, the cell M2O3 contains two ions Mz+
ok, then two ions of metal in the
M layer must be connected with three penetrating ions of oxygen O
2-ok respectively, to form a complex
M2O3 and to compose the current .
Thus, with the formation of each cell M2O3,
layer loses not two, but five ions of metal, from which three prove to be excess.Their departure from the
layer M implements balance of space,
compensating for the difference in specific volumes for each metal ion in the lattice of a metal oxide. Therefore in the passivating layer the intensive transfer of cations Mz+
ok by the mechanism of
hopping migration occurs. The surface MO is their intensive source, concentration of Nmv2 vacancies Vom in (6) is small, the relation of stationary values of currents m and ibo equal 3/2.
The total current is equal to the sum
or, accordingly (6),(3)
The current of the formation of oxide is
equal Every second on 1cm² of the
plane MO there is a number of cellsoccurs, which at zm = 3 be equal
If the stoichiometry of oxide is different than the previous one, then it will change numerical coefficients . In the general case for the cell MAOB we have
1. Vetter, K. Z. Electrochemist. 1951,55, 274;
2. Popov, Y.A. Electrochemist.1985,21, 1496;